45 (1972/73) 171-173. © NORTH-HOLLANDPUBLISHINGCO.,AMSTERDAM
LETTERS TO THE EDITORS - LETTRES AUX REDACTEURS M E A S U R E M E N T S ABOUT THE EFFECT OF GRAIN BOUNDAI~IES ON THE ELECTRICAL R E S I S T I V I T Y OF U R A N I U M D I O X I D E
W. SCHIKARSKI and G. ONDRACEK Institut ]i~r Angewandte Reaktorphysik, Institut ]i~r Material- und Festk6rper]orschung, Kern]orschungszentrum Karlsruhe, Germany
Received 10 September 1972
One of the reasons for the scattering in electrical resistivity data of UOe (up to 4 orders of magnitude at room temperature 1)) m a y be the difference in grain size. To find out to what extent grain boundaries can affect the U02 electrical resistivity the following measurements have been made. Two types of UO~ specimens having different grain sizes have been used,
the chemical analysis and stoichiometry of which were very similar (UO ratios: 1.96 for coarser grain; 1.98 for finer grain). Starting with the same powder, the compacts have been prepared by extrusion (£ = I0.69 g/cma_~97.6% TD). Different heat treatments led to the different microstructures shown in fig. 1. A rough stereometric analysis using Tomkeiff's
Fig. 1. Microstructure of coextruded UO2 with different grain size; etchant: HCL + HNO8 (l:l). ×450 171
W. S C I - I I K A R S K I A ~ D G. O N D R A C E K
Lattice defects, however, would create an effect opposite to that shown in fig. 2: the finer grained material should have the higher resistivity because of the higher concentration of lattice defects. Consequently, one can assume that the difference in the electrical resistivity shown here comes from the different grain size. Because of the high electrical resistivity of the UO2 crystallites the conductivity of the bulk material is improved by the grain boundaries. These results were observed for polycrystalline NaC1 [ref. a)] as well as for A1203 [ref. 4)], although in the latter case of AI2Oa other workers 5) have reported low grain boundary conductivity. Both results, higher as well as lower grain boundary conductivity, can be explained in terms of "binder material" in the grain boundaries of A120~ changing the electron affinity between the grain boundary and the crystal 6, 7). No conclusion can be drawn from the present results as to whether this effect occurs in U02. In spite of the clear results here, it cannot be
( L = measured mean intercept length) shows that the total internal surface (grain boundary area) per unit test volume of UOe (Sv) is approximately twice as large in the fine grained U02 as in the coarser one (fig. 1). Three specimens of each type of microstructure have been used for measuring the temperature dependence of the electrical resistivity. The resulting curves are shown in fig. 2 demonstrating that the electrical resistivity of the coarser grained U02 is approximately one order of magnitude higher than that of the finer grained UOe at all temperatures in the measured range. Due to the different heat treatments of the specimens they should also have different amounts of lattice defects. T h i s - a s well as the different m i e r o s t r u c t u r e - c o u l d be the reason for the difference in the electrical resistivity.
iner grain 0
o ._ 1=O
temperature (°C) Fig. 2.
E l e c t r i c a l r e s i s t i v i t y of UO2 s p e c i m e n s w i t h different g r a i n size.
stated generally, that the grain boundary conductivity of U02 at lower temperatures is always higher than that of the crystals.
Acknowledgements The authors gratefully acknowledge the help of Mr. Bfirkin and Mr. Rfihl in this work.
References 1) J. S. Touloukian, Thermophysieal Properties of High Temperature Solid Materials, vol. 4 (The MeMillan Company, New York, 1967) '~) E. E. Underwood, Quantitative Stereology (Addison Wesley, London, 1970) p. 34 3) H. C. Graham, N. M. Tallan and R. Russell, J. Am. Ceram. Soe. 50 (1967) 156 4) J. Cohen, Am. Ceram. Soe. Bull. 38 (1959) 441 ~) J. F. Florio, J. Am. Ceram. Soe. 43 (1960) 262 6) O. Vv~. Peters, J. Am. Ceram. Soe. 48 (1965) 220 ~) D. W. Peters, J. Am. Ceram. Sos. 48 (1965) 650